Microsoft Word - Young's modulus-arxivSpectroscopy
Department of Physics, Sogang University, Seoul 121-742,
AUTHOR EMAIL ADDRESS: [email protected]
; [email protected]
ABSTRACT: The Young’s modulus of graphene is estimated by measuring
the strain applied by a
pressure difference across graphene membranes using Raman
spectroscopy. The strain induced on
pressurized graphene balloons can be estimated directly from the
peak shift of the Raman G band. By
comparing the measured strain with numerical simulation, we
obtained the Young’s modulus of
graphene. The estimated Young’s modulus values of single- and
bi-layer graphene are 2.4±0.4 TPa and
2.0±0.5 TPa, respectively.
The mechanical properties of graphene are interesting research
subjects because its Young's modulus
and strength are known to be extremely high. Owing to these
properties, graphene is a promising
candidate for applications in nanomechanical systems.1–3
Determination of such mechanical properties
of graphene in nanometer scale is an important issue not only for
applications in nanomechanics but
also in studying fundamental physical properties. Values of ~1 TPa
for the Young's modulus have been
reported in mechanically exfoliated graphene samples by the
nanoindentation technique using an atomic
force microscopy and by the constant-N blister test.4,5 In this
work, we take a different approach and
estimate the Young’s modulus of graphene by measuring directly the
strain applied to a graphene
membrane under a differential pressure using Raman spectroscopy.
Since graphene is impermeable to
any gas,6 it can sustain a differential pressure of several
bars.5–7 By applying such a differential pressure
on a graphene membrane held over a circular aperture, a graphene
balloon is formed with a biaxial
strain applied at the center of the circular membrane. Raman
spectroscopy is a very powerful tool for
investigating the intrinsic properties of graphene.8–17 Especially,
the Raman spectrum of graphene is
very sensitive to mechanical deformations. Recent experiments
demonstrated that both the Raman G
and 2D bands red-shift and split into two peaks each under uniaxial
strain.18–21 Therefore, strain on a
graphene membrane can be measured by Raman spectroscopy very
accurately. By measuring the strain
induced on pressurized graphene balloons by Raman spectroscopy and
comparing the strain with a
numerical calculation based on the finite element method, we could
deduce the Young’s modulus of
graphene layers. This method can provide valuable information on
the intrinsic properties of graphene
and can be applied to other 2-dimensional materials for
investigating their mechanical properties.
Graphene samples were prepared on pre-patterned silicon substrates
covered with a 300-nm thick
SiO2 layer. The substrates were patterned with round holes by
photolithography and dry etching. The
depth of a hole is ~5 µm, and the diameters are 2.0, 3.1, 4.2, 5.3,
6.4, and 7.3 µm. The samples were
prepared directly on cleaned substrates by mechanical exfoliation
from natural macrocrystalline
graphite flakes (NGS Naturgraphit GmbH, Germany). The samples were
placed into a vacuum chamber
to make pressure difference across the graphene membrane.
The Raman measurements were performed with the 514.5-nm (2.41 eV)
line of an Ar ion laser. The
laser beam was focused onto the graphene sample by a 40× microscope
objective lens (N.A. 0.65)
through a quartz window. The scattered light was collected and
collimated by the same objective,
dispersed with a Jobin-Yvon Triax 550 spectrometer (1800
grooves/mm), and detected with a liquid-
nitrogen-cooled charge-coupled-device detector. The spectral
resolution was about 0.7 cm–1. The
focused beam size was measured with the razor-edge method and the
spatial resolution was ~1 μm. The
laser intensity was kept below 0.5 mW to avoid local heating
induced by the laser. For the Raman
scanning image, a spectrum was measured at each position of the
sample, raster-scanned in a rectangle
with 30×30 points in 0.3-μm steps.
Figure 1(a) shows the schematic diagram of the experimental setup.
In the vacuum chamber, a
pressure difference across the graphene membrane is applied by
pumping out the vacuum chamber. This
pressure difference makes the graphene membrane bulge upward like a
balloon. A scanning electron
microscope (SEM) image of a sample measured in vacuum is shown in
Figure 1(b). Because samples
tend to be damaged by the electron beam, the samples used for the
SEM measurements were from a
different batch than those for Raman measurements. This image
clearly shows that the graphene
membrane bulges upward. The deflection of the graphene on a 6.6 μm
diameter hole estimated from the
SEM image is about ~200 nm, which is consistent with a numerical
simulation using the finite element
Raman spectroscopic measurements were performed on the single-layer
graphene sheet shown in Fig.
2(a). The single Lorentzian shape of the 2D band in Fig.2(c) in the
supported region indicated that the
sample is clearly a single layer.22,23 But in the suspended region,
some asymmetry of the 2D band is
observed. It is consistent with the previously reported data for
the suspended single layer graphene
sample.24 At atmospheric pressure, the G peak position in the
supported region outside the hole is
substantially blue-shifted with respect to the suspended region
(Fig. S1), and the integrated intensity
ratio of the Raman 2D to G band is about 4. These and the narrow
linewidth of the G peak indicate that
the supported graphene is highly doped.10,11 It is well known that
graphene on SiO2/Si substrates can be
strongly doped.12 At the center of the hole, the peak position of
the G band is about 1581 cm–1 and the
intensity of Raman G band is very small relative to that of the 2D
band, with the intensity ratio of
Raman 2D to G band ~11, which indicates that the suspended part of
the graphene sample is minimally
doped.24,25 Furthermore, the peak position indicates that the
initial residual tension induced by Van der
Waals force between graphene and edges of the hole is very small.6
This implies that our sample is
suitable for investigating the intrinsic properties of undoped
When the chamber is evacuated, there are no distinctive changes in
the supported region. On the
other hand, the Raman spectrum from the center of the suspended
graphene is red-shifted in vacuum
[Fig. 2(c)]. The G peak position at the center of the hole is
shifted to ~1568 cm–1. Figure 2(b) is an
image of the G peak position of the graphene sample over a 6.4-μm
hole in vacuum. In the supported
region the frequency of the G peak is near 1591 cm–1. The G peak
position gradually red-shifts as the
probing position moves to the center of the hole with the minimum
value of ~1568 cm–1. This red-shift
is caused by the tension due to bulging of the graphene membrane.
Once the evacuation is complete, the
Raman spectrum did not change after more than 2 hours in vacuum,
and when the pressure is returned to
1 bar by letting air into the vacuum chamber, the G peak position
at the center went back to 1581 cm–1
(Fig. S2). The G peak position was reproducible after many cycles
of evacuation and vacuum release.
This is evidence that there is no appreciable leakage of the gas
confined in the hole. This result is
consistent with previous reports.5,6
By measuring the shifts of the Raman G and 2D bands, we can
estimate the magnitude of the strain
on a graphene membrane.18–21 To estimate the strain from the Raman
spectrum, we use the reported
value of the Grüneisen parameter ( ) and the shear deformation
potential ( ). The used values are
0(1/ )( / ) 2.2 0.1h and 0(1 / )( / ) 0.93 0.04s 20 where 0 is the
frequency of unstrained graphene, and h and s are the hydrostatic
and shear components of the strain,
respectively. Using these values, one obtains the G phonon shift
due to biaxial strain b ,
02b b , to be 70 cm–1 per biaxial strain of 1%.16 The G peak shift
of ~13 cm–1 for the 6.4-μm
hole corresponds to a biaxial strain of ~0.19% at the center of the
graphene membrane. We measured
the changes of the Raman spectrum at the center of the hole with
various diameters. Figure 3 shows that
both the Raman G and 2D bands are red-shifted and the shifts are
dependent on the diameter of the hole.
The G peak shifts are 5.0±3.6, 8.0±2.8, 10.0±1.3 and 13.0±1.0 cm–1
for the diameters of 3.1, 4.2, 5.3
and 6.4 μm, respectively. These values in turn correspond to
biaxial strain values of 0.07±0.05,
0.11±0.04, 0.14±0.03 and 0.19±0.02%, respectively. The biaxial
strain on a graphene balloon increases
as a function of the size of the hole. Some asymmetry is observed
in the line shape of the G band from
the smallest 3.1-μm hole. Since the laser spot size, ~1 μm, is a
significant fraction of the total hole size,
the strain variation within the laser spot is large relative to the
maximum strain at the center. This strain
variation causes asymmetric line shapes for smaller holes, which
contributes to larger error bars.
We compared the obtained strain values with a numerical simulation
based on the finite element
method. The graphene membrane was modeled by a clamped circular
membrane with a linear elasticity.
It is well known that graphene has a non-linear elasticity26– 28
with a form of 2E D , where E is
the Young’s modulus, D the third-order elastic modulus, the stress,
and the uniaxial strain.4 Since
typical values of E and D are 1.0 TPa and –2.0 TPa,4 respectively,
and the maximum strain applied in
our experiments was ~0.2%, the first term is much larger than the
second term, and so the elastic
behavior of graphene may be assumed to be linear in our
experimental conditions. The confined air
inside the hole under the graphene membrane is initially at
atmospheric pressure. When the vacuum
chamber is evacuated to a pressure below 10–5 torr, the graphene
membrane bulges upward and as a
result, the volume of the confined gas increases. Because of this
effect the pressure difference across the
membrane drops slightly. If one uses the deflection of ~200 nm
estimated from the SEM image [Fig
1(b)], the pressure difference is ~0.96 atm. This value was used as
the initial estimate of the pressure
difference in the iterative procedure to find the Young’s modulus.
With the iterative fitting procedure,
the deflection converges to ~160 nm and the pressure difference to
0.97 atm. We assumed that the
Poisson’s ratio of graphene is the same as that of graphite,
0.16.29 For the thickness of the graphene
membrane, we used the interlayer spacing of graphite, 0.335 nm,30
and ignored the small thickness
change by the deflection.
Numerical simulations were performed using a commercial finite
element program, ABAQUS. The
diameter of the circular membrane is taken to be the same as the
diameter of the hole. A uniform
pressure was applied perpendicular to the membrane. As a boundary
condition, the edges of the
membrane were clamped to the circular edge of the hole. This is
reasonable since Koenig et al. recently
reported that the graphene membranes firmly adhere to the substrate
up to a pressure difference of >2.5
MPa (25 atm).5
If we use the previously reported Young’s modulus value4,5 of 1 TPa
in our simulation, the
deflection is ~220 nm and the strain at the center of the circular
membrane is ~ 0.32% for the 6.4 m
hole. This is much larger than the measured value of 0.19%. If we
instead use the Young’s modulus as a
fitting parameter to reproduce the measured strain at the center,
we obtain a Young’s modulus value of
2.4 TPa. To further confirm the consistency of our analysis, we
repeated for the different hole diameters.
We obtained Young’s modulus values of 2.7±1.2, 2.7±0.8, 2.5±0.4 and
2.4±0.3 TPa for diameters of 3.1,
4.2, 5.3 and 6.4 μm, respectively. Our estimation of the Young’s
modulus of single-layer graphene is
Figure 4 shows the calculated strain distribution on the circular
membrane using the Young’s
modulus value of 2.4 TPa. The strain in the transverse direction
does not vary much whereas the radial
strain varies a lot. At the center, a biaxial strain of 0.19% is
reproduced. Near the edge of the membrane,
the transverse and radial strains are significantly different,
resulting in a shear component. We
attempted to detect this shear component using polarized Raman
Figure 5(a) shows the change of the G peak position along the
diameter of the graphene membrane,
measured in two orthogonal polarizations. The incident laser is
polarized in the vertical direction and
the laser spot position is moved horizontally. The analyzer for the
scattered signal was set either
vertically (0°) or horizontally (90°). The G peak position is
independent of the polarization near the
center whereas a small shift is seen near the edges. Figure 5(b)
compares the Raman spectra for the two
polarizations at different positions. At the center or at 1 μm from
the center, the two spectra are almost
identical. If we use the known splitting of the G peak due to
uniaxial strain, the splitting would be 0.2
cm–1 corresponding to a uniaxial strain of 0.01% at 1 μm from the
center, which is much smaller than
the width of the G peak. At the position of 2 μm away from the
center, a small relative shift of the G
peak for the two polarizations is observed. The uniaxial component
of the strain at this position is
0.05% from our simulation. This would give a G peak splitting of
1.0 cm–1, which is consistent with
what is seen in Fig. 5(b). At 3 μm away from the center, the laser
spot (~1 μm) covers both the
suspended and the supported regions, resulting in larger linewidths
and asymmetric line shapes.
We also performed the same experiment on a bilayer graphene sample.
The bilayer graphene sample
fully covered a 7.3-μm diameter hole. When the vacuum chamber is
evacuated, the G peak position is
shifted from 1581 cm–1 to 1570 cm–1, which corresponds to a biaxial
strain of 0.14% (Fig. 6). Using the
same procedure as for the single layer sample, we found that the
Young’s modulus value for bilayer
graphene is 2.0±0.5. The Young’s modulus values for single- and
bi-layer graphene, 2.4±0.4 TPa and
2.0±0.5 TPa, respectively, can be compared with that of graphite
1.02 TPa.29 (The data for a 4-layer
graphene sample is also included in Supporting Information.) This
seems reasonable if one considers
the fact that the Grüneisen parameters for graphene and graphite
are 2.2 0.1 and 1.06,
respectively.20,31 Since the Grüneisen parameter is closely related
to elastic properties, a correlation
between the Grüneisen parameter and the Young’s modulus is
Our estimations for the Young’s modulus are significantly larger
than the reported values in the
literature, ~1 TPa.4,5 A probable explanation is that the Young’s
modulus may not be constant in
different strain ranges. For example, Lee et al. fitted their data
mostly in the range of 0 to 5% of strain
with a model assuming a linear behavior to obtain the Young’s
modulus value of 1.0 TPa for single
layer graphene. Koenig et al. on the other hand, fitted their data
in the range of 0.25 to 0.5 MPa (2.5 to 5
atm) with a linear model to obtain the Young’s modulus for 1-5
layer graphene. In both cases, if
graphene has a significant softening at higher strain ranges, the
estimated Young’s modulus could be
smaller than the value estimated in the small strain range. In our
work, the maximum strain was only
0.19%, at least an order of magnitude smaller than the maximum
strain in previous work. The behavior
at even lower strain was inspected by repeating the measurements as
a function of the pressure in the
vacuum chamber between 0 and 1 atm. (See Figures S4 and S5 in
Supporting Information.) Although
accurate quantitative analysis is not possible due to the large
uncertainty caused by small Raman peak
shifts, the estimated Young’s modulus value is consistently larger
than the previous reports.
In conclusion, we found that the Young’s modulus values of single-
and bi-layer graphene are
2.4±0.4 TPa and 2.0±0.5 TPa, respectively. Comparison with previous
estimates suggests that the linear
Young’s modulus value may depend on the strain range and is larger
in small strain ranges.
ACKNOWLEDGMENT: We thank H. Kim and S. W. Lee for the SEM
measurements. This work
was supported by the National Research Foundation (NRF) grants
funded by the Korean government
(MEST) (No. 2011-0013461 and No. 2011-0017605). This work was also
supported by a grant (No.
2011-0031630) from the center for Advanced Soft Electronics under
the Global Frontier Research
Program of MEST.
Supporting Information Available: Raman G peak position as a
function of the position along the
center line of the hole, the repeatability data, Raman spectra
using different excitation energies, Raman
spectra measured at different pressures (0~1 bar), Young’s modulus
estimated at different pressures,
Raman spectra for a 4-layer sample, and Young’s modulus as a
function of the number of layers. This
material is available free of charge via the internet at
Figure 1. (a) Schematic diagram of the experimental setup. (b)
Scanning electron microscope (SEM)
image of a graphene membrane in vacuum, taken at an oblique angle.
Two bubbles with different
diameters (3.6 and 6.6 μm), formed by the pressure difference
between inside and outside of the hole,
Figure 2. (a) Optical microscope image of a graphene sample on a
pre-patterned SiO2/Si substrate. The
bright region corresponds to a thick part of the sample, and the
faintly darker area next to it corresponds
to the single layer region. (b) Raman map of the G peak position of
a single-layer graphene balloon on
the 6.4 μm hole. (c) Raman spectra measured at the center of the
6.4 μm hole and at a supported region
of a single-layer sample.
Figure 3. Comparison of the Raman (a) G band and (b) 2D band
spectra, measured from a single-layer
sample in vacuum and in ambient pressure at the center of the holes
with 3.1, 4.2, 5.3 and 6.4 μm
Figure 4. Simulated strain distribution over the single-layer
graphene membrane obtained by numerical
calculations. (Inset) Comparison of the radial and transverse
components of the strain distribution
Figure 5. (a) Shift of the G peak position due to the pressure
difference as a function of the position
along the center of the hole, measured in two orthogonal
polarizations. (b) Raman G band spectra for
two orthogonal polarizations, measured at different distances from
Figure 6. Comparison of the Raman spectra, measured from a bilayer
sample in vacuum and in ambient
pressure at the center of a 7.3-μm hole and at a supported
1. Bunch, J. S.; van der Zande, A. M.; Verbridge, S. S.; Frank, I.
W.; Tanenbaum, D. M.; Parpia, J.
M.; Craighead, H. G.; McEuen, P. L. Science 2007, 315,
2. Garcia-Sanchez, D.; van der Zande, A. M.; Paulo, A. S.;Lassagne,
B.; McEuen, P. L.; Bachtold, A.
Nano Lett. 2008, 8, 1399–1403.
3. Chen, C.; Rosenblatt S.; Bolotin K. I.; Kalb, W.; Kim, P.;
Kymissis, I.; Stormer, H. L.; Heinz, T.
F.; Hone, J. Nat. Nanotechnol. 2009, 4, 861–867.
4. Lee, C.; Wei, X.; Kysar, J. W.; Hone, J. Science 2008, 321,
5. Koenig, S. P.; Boddeti, N. G.; Dunn, M. L.; Bunch, J. S. Nat.
Nanotechnol. 2010, 6, 543–546.
6. Bunch, J. S.; Verbridge, S. S.; Alden, J. S.; van der Zande, A.
M.; Parpia, J. M.; Craighead, H. G.;
McEuen, P. L. Nano Lett. 2008, 8, 2458–2462.
7. Zabel, J.; Nair, R. R.; Ott, A.; Georgiou, T.; Geim, A. K.;
Novoselov, K. S.; Casiraghi, C. Nano
Lett. 2012, 12, 617–621.
8. Ferrari, A. C.; Meyer, J. C.; Scardaci, V.; Casiraghi, C.;
Lazzeri, M.; Mauri, F.; Piscanec, S.; Jiang,
D.; Novoselov, K. S.; Roth, S.; Geim, A. K. Phys. Rev. Lett. 2006,
9. Malard, L. M.; Pimenta, M. A.; Dresselhaus, G.; Dresselhaus, M.
S. Phys. Rep. 2009, 473, 51–87.
10. Pisana, S.; Lazzeri, M.; Casiraghi, C.; Novoselov, K. S.; Geim,
A. K.; Ferrari, A. C.; Mauri, F. Nat.
Mater. 2007, 6, 198–201.
11. Yan, J.; Zhang, Y.; Kim, P.; Pinczuk, A. Phys. Rev. Lett. 2007,
12. Casiraghi, C.; Pisana, S.; Novoselov, K. S.; Geim, A. K.;
Ferrari, A. C. Appl. Phys. Lett. 2007, 91,
13. Das, A.; Pisana, S.; Chakraborty, B.; Piscanec, S.; Saha, S.
K.; Waghmare, U. V.; Novoselov, K.
S.; Krishnamurthy, H. R.; Geim, A. K.; Ferrari, A. C.; Sood, A. K.
Nat. Nanotechnol. 2008, 3,
14. Balandin, A. A.; Ghosh, S.; Bao, W. Z.; Calizo, I.;
Teweldebrhan, D.; Miao, F.; Lau, C. N. Nano
Lett. 2008, 8, 902–907.
15. Lee, J.-U.; Yoon, D.; Kim, H.; Lee, S. W.; Cheong, H. Phys.
Rev. B 2011, 83, 081419(R).
16. Yoon, D.; Son, Y.-W.; Cheong, H. Nano Lett. 2011, 11,
17. Calizo, I.; Balandin, A. A.; Bao, W.; Miao, F.; Lau, C. N. Nano
Lett. 2007, 7, 2645 –2649.
18. Mohiuddin, T. M. G.; Lombardo, A.; Nair, R. R.; Bonetti, A.;
Savini, G.; Jalil, A.; Bonini, N.;
Basko, D. M.; Galiotis, C.; Marzari, N.; Novoselov, A. K.; Geim, A.
K.; Ferrari, A. C. Phys. Rev.
B 2009, 79, 205433.
19. Huang, M. Y.; Yan, H. G.; Chen, C. Y.; Song, D. H.; Heinz, T.
F.; Hone, J. Proc. Natl. Acad. Sci.
U.S.A. 2009, 106, 7304–7308.
20. Yoon, D.; Son, Y.-W.; Cheong, H. Phys. Rev. Lett. 2011, 106,
21. Frank, O.; Mohr, M.; Maultzsch, J.; Thomsen, C.; Riaz, I.;
Jalil, R.; Novoselov, K. S.; Tsoukleri,
G.; Parthenios, J.; Papagelis, K.; Kavan, L.; Galiotis, C. ACS Nano
2011, 5, 2231 –2239.
22. Gupta, A.; Chen, G.; Joshi, P.; Tadigadapa, S.; Eklund, P. C.
Nano Lett. 2006, 6, 2667–2673.
23. Yoon, D.; Moon, H.; Cheong, H.; Choi, J. S.; Choi, J. A.; Park,
B. H. J. Korean Phys. Soc. 2009,
24. Berciaud, S.; Ryu, S.; Brus, L. E.; Heinz, T. F. Nano Lett.
25. Casiraghi, C. Phys. Rev. B 2009, 80, 233407.
26. Liu, F.; Ming, P. B.; Li, J. Phys. Rev. B 2007, 76,
27. Wei, X.; Fragneaud, B.; Marianetti, C. A.; Kysar, J. W. Phys.
Rev. B 2009, 80, 205407.
28. Jiang, J.; Wang, J.; Li, B. Phys. Rev. B 2010, 81,
29. Blakslee, O. L.; Proctor, D. G.; Seldin, E. J.; Spence, G. B.;
Weng, T. J. Appl. Phys. 1970, 41,
30. Aljishi, R.; Dresselhaus, G. Phys. Rev. B 1982, 26, 4514
31. Hanfland, M.; Beister, H.; Syassen, K. Phys. Rev. B 1989, 39,
Department of Physics, Sogang University, Seoul 121-742,
AUTHOR EMAIL ADDRESS: [email protected]
Figure S1. Position of the Raman G band as a function of the
distance from the center of the hole of a
single-layer sample, measured in two orthogonal polarizations in
atmospheric pressure (red) and
Figure S2. Evolution of the Raman spectrum taken at the center of
the hole of a single-layer sample:
before the vacuum chamber is evacuated (Before), right after the
chamber is evacuated (Vacuum), after
the sample was held in vacuum for 2 hours (Vacuum 2h), and after
the chamber pressure was raised to
atmospheric pressure (After). This illustrates that the pressure
difference is maintained for at least 2
hours in vacuum, and there is minimal escape of the gas from the
graphene balloon during the cycle.
Figure S3. Raman spectra measured at the center of the 6.4 µm hole
at 1 atm. (unstrained) and in
vacuum (strained). Three different laser lines were used (441.6-nm
line of a He-Cd laser, 488- and
514.5-nm lines of an Ar ion laser). The peak shift is almost the
same for all laser lines.
Figure S4. Raman spectra measured at the center of the 6.4 µm hole
at different pressures.
Figure S5. Young’s modulus values estimated from Raman measurements
at different pressure
differences (Fig. S4).
Figure S6. Comparison of the Raman spectra, measured from a 4-layer
sample in vacuum and in
ambient pressure at the center of a 7.3-µm hole and at a supported
Figure S7. Estimated Young’s modulus as a function of the number of
layers. Young’s modulus
decreases as the number of layers increases.